#------------------------------------------------------------------------------
#$Date: 2016-02-16 22:30:59 +0200 (Tue, 16 Feb 2016) $
#$Revision: 176467 $
#$URL: svn://www.crystallography.net/cod/cif/4/00/13/4001332.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4001332
loop_
_publ_author_name
'Ehora, Ghislaine'
'Daviero-Minaud, Sylvie'
'Colmont, Marie'
'André, Gilles'
'Mentré, Olivier'
_publ_section_title
;
 Ba2Co9O14:  New Inorganic Building Blocks with Magnetic Ordering
 through Super-Super Exchanges Only
;
_journal_issue                   9
_journal_name_full               'Chemistry of Materials'
_journal_page_first              2180
_journal_paper_doi               10.1021/cm062897q
_journal_volume                  19
_journal_year                    2007
_chemical_formula_moiety         Ba2Co9O14
_chemical_formula_sum            'Ba6 Co27 O42'
_chemical_formula_weight         3087.15
_chemical_name_common            'barium cobalt oxide'
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           166
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-R 3 2"'
_symmetry_space_group_name_H-M   'R -3 m :H'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            3
_cell_length_a                   5.6963(8)
_cell_length_b                   5.6963(8)
_cell_length_c                   28.924(6)
_cell_measurement_temperature    293(2)
_cell_volume                     812.8(2)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.860
_diffrn_measured_fraction_theta_max 0.860
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0736
_diffrn_reflns_av_sigmaI/netI    0.0478
_diffrn_reflns_limit_h_max       7
_diffrn_reflns_limit_h_min       -7
_diffrn_reflns_limit_k_max       7
_diffrn_reflns_limit_k_min       -7
_diffrn_reflns_limit_l_max       36
_diffrn_reflns_limit_l_min       -36
_diffrn_reflns_number            1653
_diffrn_reflns_theta_full        28.08
_diffrn_reflns_theta_max         28.08
_diffrn_reflns_theta_min         2.11
_exptl_absorpt_coefficient_mu    20.612
_exptl_absorpt_process_details   Sadabs
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    6.307
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             1401
_exptl_crystal_size_max          0.4
_exptl_crystal_size_mid          0.3
_exptl_crystal_size_min          0.3
_refine_diff_density_max         3.090
_refine_diff_density_min         -2.490
_refine_diff_density_rms         0.452
_refine_ls_extinction_coef       0.0013(4)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.073
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     34
_refine_ls_number_reflns         251
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.073
_refine_ls_R_factor_all          0.0509
_refine_ls_R_factor_gt           0.0444
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0800P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1096
_refine_ls_wR_factor_ref         0.1120
_reflns_number_gt                222
_reflns_number_total             251
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cm062897qsi20061207_035759.cif
_cod_data_source_block           ba2co9
_cod_original_sg_symbol_H-M      R-3m
_cod_original_formula_sum        'Ba6Co27 O42'
_cod_database_code               4001332
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'y, x, -z'
'x-y, -y, -z'
'-x, -x+y, -z'
'x+2/3, y+1/3, z+1/3'
'-y+2/3, x-y+1/3, z+1/3'
'-x+y+2/3, -x+1/3, z+1/3'
'y+2/3, x+1/3, -z+1/3'
'x-y+2/3, -y+1/3, -z+1/3'
'-x+2/3, -x+y+1/3, -z+1/3'
'x+1/3, y+2/3, z+2/3'
'-y+1/3, x-y+2/3, z+2/3'
'-x+y+1/3, -x+2/3, z+2/3'
'y+1/3, x+2/3, -z+2/3'
'x-y+1/3, -y+2/3, -z+2/3'
'-x+1/3, -x+y+2/3, -z+2/3'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'-y, -x, z'
'-x+y, y, z'
'x, x-y, z'
'-x+2/3, -y+1/3, -z+1/3'
'y+2/3, -x+y+1/3, -z+1/3'
'x-y+2/3, x+1/3, -z+1/3'
'-y+2/3, -x+1/3, z+1/3'
'-x+y+2/3, y+1/3, z+1/3'
'x+2/3, x-y+1/3, z+1/3'
'-x+1/3, -y+2/3, -z+2/3'
'y+1/3, -x+y+2/3, -z+2/3'
'x-y+1/3, x+2/3, -z+2/3'
'-y+1/3, -x+2/3, z+2/3'
'-x+y+1/3, y+2/3, z+2/3'
'x+1/3, x-y+2/3, z+2/3'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Ba1 Ba 0.3333 0.6667 0.54949(3) 0.0086(5) Uani 1 6 d S
Co1 Co 0.0000 0.0000 0.58669(7) 0.0045(6) Uani 1 6 d S
Co2 Co 0.0000 0.0000 0.5000 0.0050(7) Uani 1 12 d S
Co3 Co 0.6667 0.3333 0.56695(8) 0.0057(6) Uani 1 6 d S
Co4 Co 0.8333 0.1667 0.6667 0.0042(6) Uani 1 4 d S
Co5 Co 1.3333 0.6667 0.6667 0.0057(8) Uani 1 12 d S
O1 O 0.2985(13) 0.1493(7) 0.5439(2) 0.0077(16) Uani 1 2 d S
O2 O 1.0000 0.0000 0.6999(4) 0.004(2) Uani 1 6 d S
O3 O 0.9732(13) 0.4866(6) 0.7043(2) 0.0068(15) Uani 1 2 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ba Ba -0.3244 2.2819 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O1 Ba1 O1 53.0(3) 1_565 3_565
O1 Ba1 O1 119.69(3) 1_565 2
O1 Ba1 O1 66.8(3) 3_565 2
O1 Ba1 O1 66.8(3) 1_565 2_665
O1 Ba1 O1 119.69(3) 3_565 2_665
O1 Ba1 O1 170.6(3) 2 2_665
O1 Ba1 O1 170.6(3) 1_565 .
O1 Ba1 O1 119.69(3) 3_565 .
O1 Ba1 O1 53.0(3) 2 .
O1 Ba1 O1 119.69(3) 2_665 .
O1 Ba1 O1 119.69(3) 1_565 3_665
O1 Ba1 O1 170.6(3) 3_565 3_665
O1 Ba1 O1 119.69(3) 2 3_665
O1 Ba1 O1 53.0(3) 2_665 3_665
O1 Ba1 O1 66.8(3) . 3_665
O1 Ba1 O3 94.66(14) 1_565 25_666
O1 Ba1 O3 123.60(16) 3_565 25_666
O1 Ba1 O3 123.60(16) 2 25_666
O1 Ba1 O3 59.92(17) 2_665 25_666
O1 Ba1 O3 94.66(14) . 25_666
O1 Ba1 O3 59.92(17) 3_665 25_666
O1 Ba1 O3 123.60(16) 1_565 27_446
O1 Ba1 O3 94.66(14) 3_565 27_446
O1 Ba1 O3 59.92(17) 2 27_446
O1 Ba1 O3 123.60(16) 2_665 27_446
O1 Ba1 O3 59.92(17) . 27_446
O1 Ba1 O3 94.66(14) 3_665 27_446
O3 Ba1 O3 63.9(2) 25_666 27_446
O1 Ba1 O3 59.92(17) 1_565 26_466
O1 Ba1 O3 59.92(17) 3_565 26_466
O1 Ba1 O3 94.66(13) 2 26_466
O1 Ba1 O3 94.66(14) 2_665 26_466
O1 Ba1 O3 123.60(16) . 26_466
O1 Ba1 O3 123.60(16) 3_665 26_466
O3 Ba1 O3 63.9(2) 25_666 26_466
O3 Ba1 O3 63.9(2) 27_446 26_466
O1 Ba1 O1 114.71(8) 1_565 21_556
O1 Ba1 O1 89.25(13) 3_565 21_556
O1 Ba1 O1 57.0(2) 2 21_556
O1 Ba1 O1 114.71(8) 2_665 21_556
O1 Ba1 O1 57.0(2) . 21_556
O1 Ba1 O1 89.25(13) 3_665 21_556
O3 Ba1 O1 145.84(8) 25_666 21_556
O3 Ba1 O1 108.44(18) 27_446 21_556
O3 Ba1 O1 145.84(8) 26_466 21_556
O1 Ba1 O1 57.0(2) 1_565 20_566
O1 Ba1 O1 57.0(2) 3_565 20_566
O1 Ba1 O1 89.25(13) 2 20_566
O1 Ba1 O1 89.25(13) 2_665 20_566
O1 Ba1 O1 114.71(8) . 20_566
O1 Ba1 O1 114.71(8) 3_665 20_566
O3 Ba1 O1 145.84(8) 25_666 20_566
O3 Ba1 O1 145.84(8) 27_446 20_566
O3 Ba1 O1 108.44(17) 26_466 20_566
O1 Ba1 O1 57.77(19) 21_556 20_566
O1 Ba1 O1 89.25(13) 1_565 19_666
O1 Ba1 O1 114.71(8) 3_565 19_666
O1 Ba1 O1 114.71(8) 2 19_666
O1 Ba1 O1 57.0(2) 2_665 19_666
O1 Ba1 O1 89.25(13) . 19_666
O1 Ba1 O1 57.0(2) 3_665 19_666
O3 Ba1 O1 108.44(18) 25_666 19_666
O3 Ba1 O1 145.84(8) 27_446 19_666
O3 Ba1 O1 145.84(8) 26_466 19_666
O1 Ba1 O1 57.8(2) 21_556 19_666
O1 Ba1 O1 57.8(2) 20_566 19_666
O1 Co1 O1 83.1(3) 3 .
O1 Co1 O1 83.1(3) 3 2
O1 Co1 O1 83.1(3) . 2
O1 Co1 O3 96.2(2) 3 26_456
O1 Co1 O3 96.2(2) . 26_456
O1 Co1 O3 179.0(3) 2 26_456
O1 Co1 O3 179.0(3) 3 27_446
O1 Co1 O3 96.2(2) . 27_446
O1 Co1 O3 96.2(2) 2 27_446
O3 Co1 O3 84.6(3) 26_456 27_446
O1 Co1 O3 96.2(2) 3 25_556
O1 Co1 O3 179.0(3) . 25_556
O1 Co1 O3 96.2(2) 2 25_556
O3 Co1 O3 84.6(3) 26_456 25_556
O3 Co1 O3 84.6(3) 27_446 25_556
O1 Co1 Co2 50.0(2) 3 .
O1 Co1 Co2 50.0(2) . .
O1 Co1 Co2 50.0(2) 2 .
O3 Co1 Co2 129.03(19) 26_456 .
O3 Co1 Co2 129.03(19) 27_446 .
O3 Co1 Co2 129.03(19) 25_556 .
O1 Co1 Co4 138.24(13) 3 3_665
O1 Co1 Co4 94.6(2) . 3_665
O1 Co1 Co4 138.24(13) 2 3_665
O3 Co1 Co4 42.42(13) 26_456 3_665
O3 Co1 Co4 42.42(13) 27_446 3_665
O3 Co1 Co4 86.4(2) 25_556 3_665
Co2 Co1 Co4 144.59(3) . 3_665
O1 Co1 Co4 138.24(13) 3 1_455
O1 Co1 Co4 138.24(13) . 1_455
O1 Co1 Co4 94.6(2) 2 1_455
O3 Co1 Co4 86.4(2) 26_456 1_455
O3 Co1 Co4 42.42(12) 27_446 1_455
O3 Co1 Co4 42.42(12) 25_556 1_455
Co2 Co1 Co4 144.59(3) . 1_455
Co4 Co1 Co4 60.23(4) 3_665 1_455
O1 Co1 Co4 94.6(2) 3 2_545
O1 Co1 Co4 138.24(13) . 2_545
O1 Co1 Co4 138.24(13) 2 2_545
O3 Co1 Co4 42.42(13) 26_456 2_545
O3 Co1 Co4 86.4(2) 27_446 2_545
O3 Co1 Co4 42.42(13) 25_556 2_545
Co2 Co1 Co4 144.59(3) . 2_545
Co4 Co1 Co4 60.23(4) 3_665 2_545
Co4 Co1 Co4 60.23(4) 1_455 2_545
O1 Co1 Ba1 55.68(3) 3 1_545
O1 Co1 Ba1 55.68(3) . 1_545
O1 Co1 Ba1 121.9(2) 2 1_545
O3 Co1 Ba1 57.14(18) 26_456 1_545
O3 Co1 Ba1 124.40(3) 27_446 1_545
O3 Co1 Ba1 124.40(3) 25_556 1_545
Co2 Co1 Ba1 71.88(4) . 1_545
Co4 Co1 Ba1 88.75(2) 3_665 1_545
Co4 Co1 Ba1 143.52(6) 1_455 1_545
Co4 Co1 Ba1 88.75(2) 2_545 1_545
O1 Co1 Ba1 55.68(3) 3 1_445
O1 Co1 Ba1 121.9(2) . 1_445
O1 Co1 Ba1 55.68(3) 2 1_445
O3 Co1 Ba1 124.40(3) 26_456 1_445
O3 Co1 Ba1 124.40(3) 27_446 1_445
O3 Co1 Ba1 57.14(18) 25_556 1_445
Co2 Co1 Ba1 71.88(4) . 1_445
Co4 Co1 Ba1 143.52(6) 3_665 1_445
Co4 Co1 Ba1 88.75(2) 1_455 1_445
Co4 Co1 Ba1 88.75(2) 2_545 1_445
Ba1 Co1 Ba1 110.79(4) 1_545 1_445
O1 Co2 O1 180.000(2) 19_556 .
O1 Co2 O1 81.9(3) 19_556 20_556
O1 Co2 O1 98.1(3) . 20_556
O1 Co2 O1 98.1(3) 19_556 2
O1 Co2 O1 81.9(3) . 2
O1 Co2 O1 180.0(3) 20_556 2
O1 Co2 O1 98.1(3) 19_556 3
O1 Co2 O1 81.9(3) . 3
O1 Co2 O1 98.1(3) 20_556 3
O1 Co2 O1 81.9(3) 2 3
O1 Co2 O1 81.9(3) 19_556 21_556
O1 Co2 O1 98.1(3) . 21_556
O1 Co2 O1 81.9(3) 20_556 21_556
O1 Co2 O1 98.1(3) 2 21_556
O1 Co2 O1 180.000(1) 3 21_556
O1 Co2 Co1 130.80(18) 19_556 .
O1 Co2 Co1 49.20(19) . .
O1 Co2 Co1 130.80(18) 20_556 .
O1 Co2 Co1 49.21(18) 2 .
O1 Co2 Co1 49.21(19) 3 .
O1 Co2 Co1 130.80(19) 21_556 .
O1 Co2 Co1 49.20(18) 19_556 19_556
O1 Co2 Co1 130.80(19) . 19_556
O1 Co2 Co1 49.20(18) 20_556 19_556
O1 Co2 Co1 130.79(18) 2 19_556
O1 Co2 Co1 130.79(19) 3 19_556
O1 Co2 Co1 49.20(19) 21_556 19_556
Co1 Co2 Co1 180.0 . 19_556
O1 Co2 Ba1 127.432(9) 19_556 1_545
O1 Co2 Ba1 52.568(8) . 1_545
O1 Co2 Ba1 64.32(18) 20_556 1_545
O1 Co2 Ba1 115.68(18) 2 1_545
O1 Co2 Ba1 52.568(8) 3 1_545
O1 Co2 Ba1 127.432(9) 21_556 1_545
Co1 Co2 Ba1 66.479(15) . 1_545
Co1 Co2 Ba1 113.521(15) 19_556 1_545
O1 Co2 Ba1 52.568(8) 19_556 19_566
O1 Co2 Ba1 127.432(9) . 19_566
O1 Co2 Ba1 115.68(18) 20_556 19_566
O1 Co2 Ba1 64.32(18) 2 19_566
O1 Co2 Ba1 127.432(9) 3 19_566
O1 Co2 Ba1 52.568(8) 21_556 19_566
Co1 Co2 Ba1 113.521(15) . 19_566
Co1 Co2 Ba1 66.479(15) 19_556 19_566
Ba1 Co2 Ba1 180.00(3) 1_545 19_566
O1 Co2 Ba1 52.568(9) 19_556 19_556
O1 Co2 Ba1 127.432(9) . 19_556
O1 Co2 Ba1 52.568(9) 20_556 19_556
O1 Co2 Ba1 127.432(9) 2 19_556
O1 Co2 Ba1 64.32(18) 3 19_556
O1 Co2 Ba1 115.68(19) 21_556 19_556
Co1 Co2 Ba1 113.521(15) . 19_556
Co1 Co2 Ba1 66.479(15) 19_556 19_556
Ba1 Co2 Ba1 74.865(17) 1_545 19_556
Ba1 Co2 Ba1 105.135(17) 19_566 19_556
O1 Co2 Ba1 127.432(9) 19_556 .
O1 Co2 Ba1 52.568(9) . .
O1 Co2 Ba1 127.432(9) 20_556 .
O1 Co2 Ba1 52.568(9) 2 .
O1 Co2 Ba1 115.68(19) 3 .
O1 Co2 Ba1 64.32(18) 21_556 .
Co1 Co2 Ba1 66.479(15) . .
Co1 Co2 Ba1 113.521(15) 19_556 .
Ba1 Co2 Ba1 105.135(17) 1_545 .
Ba1 Co2 Ba1 74.865(17) 19_566 .
Ba1 Co2 Ba1 180.0 19_556 .
O2 Co3 O1 110.1(2) 25_656 2_655
O2 Co3 O1 110.1(2) 25_656 .
O1 Co3 O1 108.8(2) 2_655 .
O2 Co3 O1 110.1(2) 25_656 3_665
O1 Co3 O1 108.8(2) 2_655 3_665
O1 Co3 O1 108.8(2) . 3_665
O2 Co3 Ba1 98.73(4) 25_656 1_545
O1 Co3 Ba1 58.918(12) 2_655 1_545
O1 Co3 Ba1 58.918(12) . 1_545
O1 Co3 Ba1 151.1(2) 3_665 1_545
O2 Co3 Ba1 98.73(4) 25_656 1_655
O1 Co3 Ba1 58.918(12) 2_655 1_655
O1 Co3 Ba1 151.1(2) . 1_655
O1 Co3 Ba1 58.918(12) 3_665 1_655
Ba1 Co3 Ba1 117.74(2) 1_545 1_655
O2 Co3 Ba1 98.73(4) 25_656 .
O1 Co3 Ba1 151.1(2) 2_655 .
O1 Co3 Ba1 58.918(12) . .
O1 Co3 Ba1 58.918(13) 3_665 .
Ba1 Co3 Ba1 117.74(2) 1_545 .
Ba1 Co3 Ba1 117.74(2) 1_655 .
O2 Co3 Ba1 179.999(1) 25_656 19_666
O1 Co3 Ba1 69.9(2) 2_655 19_666
O1 Co3 Ba1 69.9(2) . 19_666
O1 Co3 Ba1 69.9(2) 3_665 19_666
Ba1 Co3 Ba1 81.27(4) 1_545 19_666
Ba1 Co3 Ba1 81.27(4) 1_655 19_666
Ba1 Co3 Ba1 81.27(4) . 19_666
O2 Co4 O2 179.998(1) 25_656 .
O2 Co4 O3 96.5(2) 25_656 27_546
O2 Co4 O3 83.5(2) . 27_546
O2 Co4 O3 96.5(2) 25_656 25_656
O2 Co4 O3 83.5(2) . 25_656
O3 Co4 O3 86.0(4) 27_546 25_656
O2 Co4 O3 83.5(2) 25_656 3_665
O2 Co4 O3 96.5(2) . 3_665
O3 Co4 O3 179.998(3) 27_546 3_665
O3 Co4 O3 94.0(4) 25_656 3_665
O2 Co4 O3 83.5(2) 25_656 .
O2 Co4 O3 96.5(2) . .
O3 Co4 O3 94.0(4) 27_546 .
O3 Co4 O3 180.0(4) 25_656 .
O3 Co4 O3 86.0(4) 3_665 .
O2 Co4 Co1 95.1(3) 25_656 1_655
O2 Co4 Co1 84.9(3) . 1_655
O3 Co4 Co1 43.15(19) 27_546 1_655
O3 Co4 Co1 43.15(19) 25_656 1_655
O3 Co4 Co1 136.85(19) 3_665 1_655
O3 Co4 Co1 136.85(19) . 1_655
O2 Co4 Co1 84.9(3) 25_656 25_556
O2 Co4 Co1 95.1(3) . 25_556
O3 Co4 Co1 136.85(19) 27_546 25_556
O3 Co4 Co1 136.85(19) 25_656 25_556
O3 Co4 Co1 43.15(19) 3_665 25_556
O3 Co4 Co1 43.15(19) . 25_556
Co1 Co4 Co1 180.0 1_655 25_556
O2 Co4 Co4 41.6(2) 25_656 3_665
O2 Co4 Co4 138.4(2) . 3_665
O3 Co4 Co4 137.87(13) 27_546 3_665
O3 Co4 Co4 93.41(17) 25_656 3_665
O3 Co4 Co4 42.13(13) 3_665 3_665
O3 Co4 Co4 86.59(17) . 3_665
Co1 Co4 Co4 120.12(2) 1_655 3_665
Co1 Co4 Co4 59.88(2) 25_556 3_665
O2 Co4 Co4 41.6(2) 25_656 2_655
O2 Co4 Co4 138.4(2) . 2_655
O3 Co4 Co4 93.41(17) 27_546 2_655
O3 Co4 Co4 137.87(13) 25_656 2_655
O3 Co4 Co4 86.59(17) 3_665 2_655
O3 Co4 Co4 42.13(13) . 2_655
Co1 Co4 Co4 120.12(2) 1_655 2_655
Co1 Co4 Co4 59.88(2) 25_556 2_655
Co4 Co4 Co4 60.0 3_665 2_655
O2 Co4 Co5 90.000(2) 25_656 1_445
O2 Co4 Co5 90.000(2) . 1_445
O3 Co4 Co5 133.01(19) 27_546 1_445
O3 Co4 Co5 46.99(19) 25_656 1_445
O3 Co4 Co5 46.99(19) 3_665 1_445
O3 Co4 Co5 133.01(19) . 1_445
Co1 Co4 Co5 90.0 1_655 1_445
Co1 Co4 Co5 90.0 25_556 1_445
Co4 Co4 Co5 60.0 3_665 1_445
Co4 Co4 Co5 120.0 2_655 1_445
O2 Co4 Co5 90.000(2) 25_656 .
O2 Co4 Co5 90.000(2) . .
O3 Co4 Co5 46.99(19) 27_546 .
O3 Co4 Co5 133.01(19) 25_656 .
O3 Co4 Co5 133.01(19) 3_665 .
O3 Co4 Co5 46.99(19) . .
Co1 Co4 Co5 90.0 1_655 .
Co1 Co4 Co5 90.0 25_556 .
Co4 Co4 Co5 120.0 3_665 .
Co4 Co4 Co5 60.0 2_655 .
Co5 Co4 Co5 180.0 1_445 .
O3 Co5 O3 95.2(2) 27_546 25_766
O3 Co5 O3 95.2(2) 27_546 26_566
O3 Co5 O3 95.2(2) 25_766 26_566
O3 Co5 O3 180.00(19) 27_546 3_775
O3 Co5 O3 84.8(2) 25_766 3_775
O3 Co5 O3 84.8(2) 26_566 3_775
O3 Co5 O3 84.8(2) 27_546 .
O3 Co5 O3 179.998(1) 25_766 .
O3 Co5 O3 84.8(2) 26_566 .
O3 Co5 O3 95.2(2) 3_775 .
O3 Co5 O3 84.8(2) 27_546 2_755
O3 Co5 O3 84.8(2) 25_766 2_755
O3 Co5 O3 180.00(12) 26_566 2_755
O3 Co5 O3 95.2(2) 3_775 2_755
O3 Co5 O3 95.2(2) . 2_755
O3 Co5 Co4 89.999(1) 27_546 2_655
O3 Co5 Co4 137.61(11) 25_766 2_655
O3 Co5 Co4 42.39(11) 26_566 2_655
O3 Co5 Co4 90.000(2) 3_775 2_655
O3 Co5 Co4 42.39(11) . 2_655
O3 Co5 Co4 137.61(11) 2_755 2_655
O3 Co5 Co4 137.61(11) 27_546 3_775
O3 Co5 Co4 89.999(1) 25_766 3_775
O3 Co5 Co4 42.39(11) 26_566 3_775
O3 Co5 Co4 42.39(11) 3_775 3_775
O3 Co5 Co4 90.000(1) . 3_775
O3 Co5 Co4 137.61(11) 2_755 3_775
Co4 Co5 Co4 60.0 2_655 3_775
O3 Co5 Co4 137.61(11) 27_546 1_665
O3 Co5 Co4 42.39(11) 25_766 1_665
O3 Co5 Co4 90.000(1) 26_566 1_665
O3 Co5 Co4 42.39(11) 3_775 1_665
O3 Co5 Co4 137.61(11) . 1_665
O3 Co5 Co4 90.000(1) 2_755 1_665
Co4 Co5 Co4 120.0 2_655 1_665
Co4 Co5 Co4 60.0 3_775 1_665
O3 Co5 Co4 42.39(11) 27_546 .
O3 Co5 Co4 137.61(11) 25_766 .
O3 Co5 Co4 90.000(1) 26_566 .
O3 Co5 Co4 137.61(11) 3_775 .
O3 Co5 Co4 42.39(11) . .
O3 Co5 Co4 90.000(1) 2_755 .
Co4 Co5 Co4 60.0 2_655 .
Co4 Co5 Co4 120.0 3_775 .
Co4 Co5 Co4 180.0 1_665 .
O3 Co5 Co4 42.39(11) 27_546 3_765
O3 Co5 Co4 90.001(1) 25_766 3_765
O3 Co5 Co4 137.61(11) 26_566 3_765
O3 Co5 Co4 137.61(11) 3_775 3_765
O3 Co5 Co4 90.000(1) . 3_765
O3 Co5 Co4 42.39(11) 2_755 3_765
Co4 Co5 Co4 120.0 2_655 3_765
Co4 Co5 Co4 180.0 3_775 3_765
Co4 Co5 Co4 120.0 1_665 3_765
Co4 Co5 Co4 60.0 . 3_765
O3 Co5 Co4 90.001(1) 27_546 2_755
O3 Co5 Co4 42.39(11) 25_766 2_755
O3 Co5 Co4 137.61(11) 26_566 2_755
O3 Co5 Co4 90.000(2) 3_775 2_755
O3 Co5 Co4 137.61(11) . 2_755
O3 Co5 Co4 42.39(11) 2_755 2_755
Co4 Co5 Co4 180.0 2_655 2_755
Co4 Co5 Co4 120.0 3_775 2_755
Co4 Co5 Co4 60.0 1_665 2_755
Co4 Co5 Co4 120.0 . 2_755
Co4 Co5 Co4 60.0 3_765 2_755
Co1 O1 Co3 119.8(3) . .
Co1 O1 Co2 80.8(3) . .
Co3 O1 Co2 159.3(4) . .
Co1 O1 Ba1 90.57(13) . 1_545
Co3 O1 Ba1 85.65(13) . 1_545
Co2 O1 Ba1 94.72(14) . 1_545
Co1 O1 Ba1 90.57(13) . .
Co3 O1 Ba1 85.65(13) . .
Co2 O1 Ba1 94.72(14) . .
Ba1 O1 Ba1 170.6(3) 1_545 .
Co1 O1 Ba1 163.9(3) . 19_666
Co3 O1 Ba1 76.2(2) . 19_666
Co2 O1 Ba1 83.1(2) . 19_666
Ba1 O1 Ba1 90.75(13) 1_545 19_666
Ba1 O1 Ba1 90.75(13) . 19_666
Co4 O2 Co4 96.8(4) 2_645 3_765
Co4 O2 Co4 96.8(4) 2_645 .
Co4 O2 Co4 96.8(4) 3_765 .
Co4 O2 Co3 120.3(3) 2_645 25_656
Co4 O2 Co3 120.3(3) 3_765 25_656
Co4 O2 Co3 120.3(3) . 25_656
Co4 O3 Co4 95.7(3) 2_655 .
Co4 O3 Co1 94.4(2) 2_655 25_556
Co4 O3 Co1 94.4(2) . 25_556
Co4 O3 Co5 90.6(2) 2_655 .
Co4 O3 Co5 90.6(2) . .
Co1 O3 Co5 172.4(3) 25_556 .
Co4 O3 Ba1 131.91(13) 2_655 25_666
Co4 O3 Ba1 131.91(13) . 25_666
Co1 O3 Ba1 88.6(2) 25_556 25_666
Co5 O3 Ba1 83.8(2) . 25_666
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Ba1 O1 2.8578(7) 1_565
Ba1 O1 2.8578(7) 3_565
Ba1 O1 2.8578(7) 2
Ba1 O1 2.8578(7) 2_665
Ba1 O1 2.8578(7) .
Ba1 O1 2.8578(7) 3_665
Ba1 O3 2.908(6) 25_666
Ba1 O3 2.908(6) 27_446
Ba1 O3 2.908(6) 26_466
Ba1 O1 3.256(6) 21_556
Ba1 O1 3.256(6) 20_566
Ba1 O1 3.256(6) 19_666
Co1 O1 1.923(6) 3
Co1 O1 1.923(6) .
Co1 O1 1.923(6) 2
Co1 O3 1.947(7) 26_456
Co1 O3 1.947(7) 27_446
Co1 O3 1.947(7) 25_556
Co1 Co2 2.507(2) .
Co1 Co4 2.8382(18) 3_665
Co1 Co4 2.8382(18) 1_455
Co1 Co4 2.8382(18) 2_545
Co1 Ba1 3.4603(9) 1_545
Co1 Ba1 3.4603(9) 1_445
Co2 O1 1.945(7) 19_556
Co2 O1 1.945(7) .
Co2 O1 1.945(7) 20_556
Co2 O1 1.945(7) 2
Co2 O1 1.945(7) 3
Co2 O1 1.945(7) 21_556
Co2 Co1 2.507(2) 19_556
Co2 Ba1 3.5868(6) 1_545
Co2 Ba1 3.5868(6) 19_566
Co2 Ba1 3.5868(6) 19_556
Co3 O2 1.924(12) 25_656
Co3 O1 1.934(7) 2_655
Co3 O1 1.934(7) .
Co3 O1 1.934(7) 3_665
Co3 Ba1 3.3273(6) 1_545
Co3 Ba1 3.3273(6) 1_655
Co3 Ba1 3.368(2) 19_666
Co4 O2 1.904(6) 25_656
Co4 O2 1.904(6) .
Co4 O3 1.920(4) 27_546
Co4 O3 1.920(4) 25_656
Co4 O3 1.920(4) 3_665
Co4 O3 1.920(4) .
Co4 Co1 2.8382(18) 1_655
Co4 Co1 2.8382(18) 25_556
Co4 Co4 2.8482(4) 3_665
Co4 Co4 2.8482(4) 2_655
Co4 Co5 2.8482(4) 1_445
Co4 Co5 2.8482(4) .
Co5 O3 2.083(6) 27_546
Co5 O3 2.083(7) 25_766
Co5 O3 2.083(6) 26_566
Co5 O3 2.083(7) 3_775
Co5 O3 2.083(7) .
Co5 O3 2.083(6) 2_755
Co5 Co4 2.8482(4) 2_655
Co5 Co4 2.8482(4) 3_775
Co5 Co4 2.8482(4) 1_665
Co5 Co4 2.8482(4) 3_765
Co5 Co4 2.8481(4) 2_755
O1 Ba1 2.8578(7) 1_545
O1 Ba1 3.256(6) 19_666
O2 Co4 1.904(6) 2_645
O2 Co4 1.904(6) 3_765
O2 Co3 1.924(12) 25_656
O3 Co4 1.920(4) 2_655
O3 Co1 1.947(7) 25_556
O3 Ba1 2.908(6) 25_666
